Polyaniline (PANI) Composites − Preparation in Carbonated ...Goto, H.; Kawashima, H. Polyaniline...
Embed Size (px)
Transcript of Polyaniline (PANI) Composites − Preparation in Carbonated ...Goto, H.; Kawashima, H. Polyaniline...
Goto, H.; Kawashima, H. Polyaniline (PANI) Composites − Preparation in Carbonated Water, PANI/Pulp Paper Sheet, and PANI/Surfactant.FIBRES & TEXTILES in Eastern Europe 2012, 20, 1(90) 86-89.
Polyaniline (PANI) Composites − Preparation in Carbonated Water, PANI/Pulp Paper Sheet, and PANI/Surfactant
Hiromasa Goto, Hirotsugu Kawashima
Graduate School of Pure and Applied Sciences, Institute of Materials Science,
University of Tsukuba,Tsukuba, Ibaraki 305-8573, Japan
Email: [email protected]
AbstractThe polymerisation of aniline in the presence of pulp was carried out in saturated carbon-ated water in the place of sulfuric acid for the preparation of a PANI/pulp composite, and a conductive paper sheet was prepared from the composite using the papermaking technique. The surface structure and conductivity were examined. Furthermore, micro-fibre of PANI was prepared using a surfactant.
Key words: carbon dioxide, electrical conductivity, pulp, polyaniline, micro-fibre.
n IntroductionGenerally the synthesis of polyaniline (PANI) as an electrical conductive poly-mer can be carried out with chemical or electrochemical polymerisation. Recent-ly the polymerisation of aniline mono-mer in carbonated water was performed to obtain polyaniline . Moreover the preparation of a PANI/pulp composite with sulfuric acid has also been per-formed, and a conducting paper was pre-pared from the PANI/pulp composite by a papermaking technique . The combi-nation of textile and conducting polymer can open a new avenue for textile materi-als science [3 - 7]. In the present research, a PANI/pulp composite material was syn-thesised in carbonated water with a view to conductive textile applications. Here, carbonated water was employed for the acid conditioning of aniline polymerisa-tion instead of sulfuric acid, which was possibly the first attempt at the prepara-tion of a PANI based composite in car-bonated water. After the reaction the po-lymerisation water contained no sulphu-ric acid, which can be an advantage for industry with respect to the environment.
The PANI/pulp composite was fabri-cated by a papermaking method for the preparation of a conductive paper sheet. Furthermore, polyaniline micro-fibre was prepared using a surfactant by means of the bottom up method. The materials processing techniques used in this study
and several pieces of dry paper, pressed to remove moisture, and then the PANI/pulp composite sheet was dried.
The composite sheet was immersed in ammonia/water to neutrise the PANI component in the paper sheet, during which the colour of the surface changed from dark emerald green to dark blue, and was then dried at room temperature. The reduction treatment in ammonia produces a composite paper sheet with insulating properties.
The preparation of PANI/SDBS was car-ried out as follows: SDBS (25 mg), wa-ter (0.5 g), and N-methyl-2-pyrrolidone (0.2 g) were added to a suspension (10 mg, conc. < 2.5%) of polyaniline (as polymerisation solution) in CO2, and the mixture was ultrasonicated for 30 min. The solvents in the solution were then evaporated using a hot stage at ca. 100 °C to yield a dark emerald green material. Visual inspection of the dark emerald green colour indicated that the resultant material consists of PANI.
TechniqueIR absorption spectra for the polymers were obtained using a Jasco IR 550 spectrometer with the KBr method. SEM observation was performed with a JEOL JSM-521. At room temperature, the electrical conductivity of the polymers was measured by using a Mitsubishi Lowrester-GP MCTP-T610 with MCP-TP06P probe and a Hioki SM-8213. Circular differential interference con-trast optical microscopy (C-DIM) obser-vations were carried out using a Nikon ECLIPS LV 100 high-resolution micro-scope with circular polariser and Nikon CFIUW lenses. The composition of the PANI/pulp composite paper was evaluat-ed by X-ray photoelectron spectroscopy (XPS, JPS-9010TR, JEOL).
may contribute to the production of new conductive materials.
n ExperimentalMaterialsAniline (Tokyo Kasei, TCI), and water were distilled prior to use. Ammonium persulphate (APS; Kanto Chemicals, Japan) was used as received. For the present research saturated carbonated water was prepared by the injection of high pressure CO2 gas into the distilled water in a small stainless steel jar prior to the polymerisation of aniline. A mem-brane filter (Toyo filter paper) was ho-mogenised in an appropriate amount of carbonated water to prepare dispersed pulp fibres. Furthermore sodium do-decylbenzene sulphonate (SDBS) was obtained from TCI.
SynthesisThe PANI/pulp composite was prepared by the following method: Aniline (3.0 g) and pulp (3.0 g) were added to 240 mL of saturated carbonated water in an Er-lenmeyer flask at room temperature. The mixture was stirred for 30 min at 0 °C. APS (9.0 g) was then slowly added to the mixture at 0 °C. After 24 h, the mixture was filtered, washed with a large volume of water for 12 h, filtered again, and the resultant material was then washed with a large volume of methanol for 12 h. Af-ter filtration, the PANI/pulp mixture was dried. Next a PANI/pulp composite paper sheet was prepared using a papermaking technique . The composite fibres were dispersed in a large volume of water, and the suspension was then filtered using a large Büchner funnel. A wet dark-col-oured PANI/pulp paper layer appeared on the filter paper of the Büchner fun-nel. The wet PANI/pulp layer was sand-wiched between a thin aluminium plates
87FIBRES & TEXTILES in Eastern Europe 2012, Vol. 20, No. 1 (90)
n Results and discussionIRThe IR spectra of the pulp and PANI/pulp composite paper in both forms the pristine and deprotonated using ammonia are shown in Figure 1. The pulp exhib-its absorption bands in the high energy region due to νOH stretching vibration at 3378 cm−1 and νCH at 2897 cm−1. In contrast, the polymer composite paper (pristine) displays no clear absorption bands related to νCH and νOH stretch-ing, due to overlapping with the polymer absorptions in the same infrared region. The pristine PANI sample has an intense absorption band at 1580 cm−1 derived from the quinoid (Q) structure, as com-pared with that due to the benzenoid (B) structure at 1510 cm−1. This is character-istic of IR absorptions of emeraldine salt, while the deprotonated PANI/pulp (treat-ed with ammonia) displays relatively weak Q structure absorption, indicative of the emeraldine base.
Electrical conductivityThe pristine PANI/pulp composite paper sheet displays a rapid decrease (<5 s) in resistance from >10 MΩ to ca. 1.35 kΩ upon in situ vapour phase doping with hydrochloric acid. In this case, hydro-chloric acid functions as an agent for further protonation, and a salt form (con-ductive state) is produced from the emer-aldine base of PANI in the composite, as indicated by the quick decrease in resist-ance (increase in conductivity).
Surface imageThe pristine PANI/pulp composite paper sheet has a smooth surface of dark emer-ald green colour. Although a PANI/pulp composite sheet was obtained with sul-
shows the change in conductivity with the bend angle. The sample was doped with vapour phase of HCl before the conductivity measurements. The conduc-tivity measurements were carried out by the two-probe method along the sample length. The inset of Figure 3 shows an il-lustration of the bend degree. An increase in the bend degree allows an increase in electrical conductivity. This can be due to the fact that the bending process made the paper dense, which partly improves the conduction pass, resulting in an in-crease in electrical conductivity.
furic acid in a previous study , this re-sult demonstrates that a conductive sheet can be prepared by using carbon dioxide instead of acid regents. The low magni-fication SEM image of the PANI/paper composite paper sheet in Figure 2.a in-dicates that the PANI coated the entire sheet. The higher magnification SEM image in Figure 2.b shows fine particle agglomerates distributed over the indi-vidual fibres. The SEM images visually demonstrate that the polymerisation of the aniline monomer on the pulp sur-face is achieved in the presence of APS in saturated carbonated water. Figure 3
4000 3000 2000 1000 500Wavenumber / cm-1
Figure 1. IR ab-sorption spectra of (a) the pulp, (b) pristine PANI/pulp (emeraldine salt), and (c) PANI/pulp treated with am-monia (emeraldine base).
Figure 2. SEM image of the composite paper sheet surface at (a) 500× and (b) 6,000× magnification.
FIBRES & TEXTILES in Eastern Europe 2012, Vol. 20, No. 1 (90)88
a weak absorption signal due to these alkyl groups at 2933 cm−1 and absorp-tion bands at 1570 cm−1 and 1484 cm−1 due to the Q and B structures, respective-ly (Figure 5.b). Other absorption bands, such as 1293 cm−1 (C-N stretching of the ternary aromatic amine), 1128 cm−1 (in-plane C-H vibration of the benzene ring) and 823 cm−1 (out-of-plane C-H vibration of the benzene ring) are char-acteristic of PANI . These results sug-gest that the material obtained is a PANI/SDBS composite. Circular differential interference contrast optical microscope images of the PANI/SDBS indicate mi-crofibril structures with colour at low magnification, as shown in Figure 6.a. The PANI/SDBS composite exhibits a radial structure, like a dendrite in the neuron system, revealed at higher magni-fication (500 ×), as shown in Figure 6.b. The SEM image (2000 ×) of the PANI/SDBS composite confirms the forma-tion of a microfibril structure, as shown in Figure 6.c. An ordered structure is derived from the self-assembly process due to the aggregation properties of the surfactant [10 − 12]. This experiment demonstrates that the treatment of PANI with a surfactant enables the formation of an ordered microstructure. The elec-trical conductivity of the PANI/SDBS composite is 2.3×10−5 S/cm, evaluated by the four-probe method.
A proposed schematic illustration of the PANI/SDBS composite structure is given in Figure 6 (c, inset). The hydrophilic moiety of SDBS (anion part) and the hydrophobic alkyl group located in the outer layer and core, respectively, form the micro-fibril structure.
CompositionFigure 4.a shows the X-ray photoelec-tron spectroscopy (XPS) measurement result of the PANI/pulp. The PANI/pulp was treated with hydrazine for the prepa-ration of a completely reduced (dedoped) state of the PANI in the composite, and the sample was washed with ethanol and dried in a vacuum before the XPS meas-urement. XPS signals of nitrogen and oxygen appear at 399 eV (abundance =
= 24.36%) and 533 eV (abundance = = 75.64%), respectively. Magnification of the XPS result clearly indicates these signals, as shown in Figures 4.b, 4.c. The composition of MRUPANI/MRUCEL-LULOSE (MRU = monomer repeat unit, MRUPANI = C6H5N, MRUCELLULOSE = C6H10O5) of the composite is calcu-lated to be ca. 15.5, obtained from the XPS data. However, this composition value was estimated for only the skin of the PANI/pulp because XPS analysis was carried out for the surface of the sample.
PANI and surfactantThe treatment of polymers with sur-factant can produce a characteristic structure, such as a sphere. In this study, the treatment of PANI with a surfactant (SDBS) was conducted to explore the preparation of an ordered structure.
Figure 5 shows the IR absorption spectra of SDBS and the resultant material. The absorption band of SDBS at 2933 cm−1 is due to the stretching vibrations of alkyl groups (CH2, and CH3) (Figure 5.a). The surfactant treated compound shows
Figure 5. IR absorption spectra of (a) so-dium dodecylbenzene sulphonate (SDBS) and (b) PANI/SDBS composite.
Figure 3. Conductivities of the PANI/pulp paper as a function of the bend degree (θ). The inset shows the bend degree. The con-ductivities were obtained by the two-probe method.
Figure 4. X-ray photoelectron spectroscopy (XPS) measurement result of the PANI/pulp sheet. Wide scan measurement (a) (At = atomic%), narrow scan measurement at nitrogen region (b), and narrow scan measurement at oxygen region (c). Inset (a) shows the molecu-lar structure of PANI and cellulose, and chemical formulas.
89FIBRES & TEXTILES in Eastern Europe 2012, Vol. 20, No. 1 (90)
n ConclusionsA PANI/pulp paper was prepared by the polymerisation of aniline in CO2 water in the presence of pulp, followed by a pa-permaking procedure. Generally, the em-ployment of a high boiling point solvent, such as N-methyl-2-pyrrolidone, and evaporation processes is required for the
Figure 6. Circular differential interference contrast optical microscopy (C-DIM) images at (a) 200× and (b) 500×, and (c) SEM image of the PANI/SDBS composite at 2000×. (Inset (c)) plausible structure of PANI/SDBS micro-fibres. SDBS = sodium dodecylbenzene sulphonate (surfactant).
Received 03.11.2010 Reviewed 20.09.2011
preparation of conductive polymer films using the casting method. On the other hand, the conductive paper sheet has ad-vantage of processability.
In this study, the surface structure, elec-trical conductivity and sensor func-tion were examined. Furthermore a PANI/surfactant composite with an or-
dered structure was prepared in a mixed solution of water. These simple and convenient methods for the preparation of a conductive organic composite may enable to produce low-cost conductive polymer materials, which may extend to industrial applications.
AcknowledgmentThe author would like to thank the Glass workshop of the Central Workshop of the University of Tsukuba for the fine glass work. H. Kawashima measured the XPS for the sample.
References 1. Goto, H. Fibres & Textiles in Eastern
Europe, 2011, 19, 15−17. 2. Goto, H. Text. Res. J., 2011, 81, 122-
127. 3. Śniechowski, M.; Łużny, W.; Djurado, D.;
Dufour, B.; Rannou, P.; Proń, A.; Bee, M.; Johnson, M.; Gonzales, M. Fibres & Textiles in Eastern Europe, 2005, 13, 96-99.
5. Fryczkowski, M.; Rom, M.; Fryczkowska, B. Fibres & Textiles in Eastern Europe, 2005, 13, 141-143.
6. Połowiński, S.; Szumilewicz, J.; Stawski, D. Fibres & Textiles in Eastern Europe, 2011, 19, 119-123.
7. Krucińska, I.; Urbaniak–Domagała, W.; Skoneczna, M.; Cosseddu, P.; Bonfiglio, A. Fibres & Textiles in Eastern Europe, 2011, 19, 78-83.
8. Rahman, N. A.; Gizdavic-Nikolaidis M.; Ray S.; Easteal A.J.; Travas-Sejdic J. Synth Met, 2010, 160, 2015-2022.
9. Tang, J.; Jing, X.; Wang, B.; Wang, F. Synth. Met.,1988, 24 231-238.
10. Landfester, K.; Montenegro, R.; Scherf, U.; Gunter, R.; Asawapirom, U.; Patil, S.; Neher, D. Kietzke, T. Adv. Mater., 2002, 14, 651–654.
11. Li, Y.; Wang, Y.; Wu, D.; Jing, X. J .Appl. Polym. Sci. 2009, 113 868–875.
12. Tada, K.; Onoda, M. Thin Solid Films, 2006, 499, 19–22.